# Performance of various density-functional approximations for … · 2018-05-24 · Performance of...

Embed Size (px)

### Transcript of Performance of various density-functional approximations for … · 2018-05-24 · Performance of...

Performance of various density-functional

approximations for cohesive properties of 64 bulk

solids

Guo-Xu Zhang 1,2, Anthony M. Reilly 1,3, Alexandre

Tkatchenko 1,4, and Matthias Scheffler 1

1 Fritz-Haber-Institut der Max-Planck-Gesellschaft, Faradayweg 4-6, 14195, Berlin,

Germany2 School of Chemistry and Chemical Engineering, Harbin Institute of Technology,

West Dazhi 92, 150001, Harbin, P. R. China3 School of Chemical Sciences, Dublin City University, Glasnevin, Dublin 9, Ireland4 Physics and Materials Science Research Unit, University of Luxembourg, L-1511

Luxembourg

E-mail: [email protected]

Abstract. Accurate and careful benchmarking of different density-functional ap-

proximations (DFAs) represents an important source of information for understanding

DFAs and how to improve them. In this work we have studied the lattice constants,

cohesive energies, and bulk moduli of 64 solids using six functionals, representing

the local, semi-local, and hybrid DFAs on the first four rungs of Jacob’s ladder.

The set of solids considered consists of ionic crystals, semiconductors, metals, and

transition-metal carbides and nitrides. To minimize numerical errors and to avoid

making further approximations, the full-potential, all-electron FHI-aims code has been

employed, and all the reported cohesive properties include contributions from zero-

point vibrations. Our assessment demonstrates that current DFAs can predict cohesive

properties with mean absolute relative errors of 0.6% for the lattice constant and 6% for

both the cohesive energy and the bulk modulus over the whole database of 64 solids.

For semiconducting and insulating solids, the recently proposed SCAN meta-GGA

functional represents a substantial improvement over the other functionals. However,

when considering the different types of solids in the set, all of the employed functionals

exhibit some variance in their performance. There are clear trends and relationships in

the deviations of the cohesive properties, pointing to the need to consider, for example,

long-range van der Waals (vdW) interactions. This point is also demonstrated by

consistent improvements in predictions for cohesive properties of semiconductors when

augmenting GGA and hybrid functionals with a screened Tkatchenko-Scheffler vdW

energy term.

Submitted to: New J. Phys.

Keywords : density-functional theory, Jacob’s ladder, cohesive properties

Performance of various density-functional approximations for cohesive properties of 64 bulk solids2

1. Introduction

Density-functional theory (DFT) [1] in the Kohn-Sham (KS) [2] framework has proven

to be a very useful tool in condensed-matter physics and quantum chemistry. [3–7]

Its favorable ratio of accuracy to computational cost makes it a powerful method

for calculating ground-state properties of large systems. Hohenberg-Kohn DFT is, in

principle, an exact theory but as the form of the exact electronic exchange-correlation

(XC) functional is unknown, a wide range of density-functional approximations (DFAs)

have been proposed.

Cohesive properties (lattice constant, cohesive energy, and bulk modulus) can be

used as probes to identify and understand the performance of each functional applied

to solid-state materials, and noticeably different performance has been reported when

using different DFAs, with significant deviations possible for a range of properties (see

e.g., [8–19]). Therefore, developing reliable and efficient XC functionals that are

applicable to a broad range of systems remains an ongoing challenge. It is especially

relevant now as DFT calculations are becoming ubiquitous and numerically reproducible.

[20] Investigating trends in predictions and deviations from experiment can help us to

improve our understanding of DFAs, as well as bulk properties themselves.

In this work, we explore the question of accuracy of DFAs on the first four rungs of

the Jacob’s ladder proposed by Perdew and Schmidt, [3,21] with each rung corresponding

to more ingredients and contributions (besides the electron density) forming the DFA,

ideally, leading to DFAs with improved accuracy. The local-density approximation

(LDA) [2] represents the first rung of Jacob’s ladder, considering only the density itself,

and therefore it is a successful approximation for systems in which the electron density

varies slowly, such as nearly free-electron metals, but is also surprisingly successful for

less-uniform systems, such as molecules and semiconductors. However, there are many

features that LDA fails to describe, with lattice constants typically being too small,

up to 5% shorter than experiment, and cohesive energies (or atomization energies in

molecules) that are very inaccurate, typically off by 20–30%. [19]

Functionals based on the generalized gradient approximation (GGA) are on the next

rung of the ladder, and represent an extension of the LDA functional by introducing

the gradient of the electron density. They are also referred to as semi-local DFAs, and

are successful in improving over LDA for certain properties. For example, they cure the

overbinding problem of LDA and predict more accurate bond lengths. However, they

show a tendency towards underbinding. [8–12,14,15]

The Perdew-Burke-Ernzerhof (PBE) [22] GGA is one of the most widely used DFAs

and many approaches (e.g., revPBE [23] and RPBE [24]) have been explored to improve

upon it. A simple modification of PBE is the PBEsol functional, [25] which differs from

PBE only in two parameters, and is designed to improve upon PBE for equilibrium

properties of bulk solids and their surfaces. By restoring the gradient expansion for

exchange, PBEsol lattice constants are systematically lower and better than PBE by

1–2%, however with the drawback of cohesive energies being less accurate. [10–14]

Performance of various density-functional approximations for cohesive properties of 64 bulk solids3

The meta-GGA (or MGGA) family [26–28] is on the third rung of Jacob’s ladder

and makes use of the kinetic-energy density in addition to the electron density and its

gradient. While some MGGAs predict cohesive properties with reasonable accuracy

for specific systems, [8–13, 29, 30] improvements in the lattice constant are often

accompanied by a worsening of the bulk modulus or the cohesive energy, or both.

The non-empirical Tao-Perdew-Staroverov-Scuseria (TPSS) [28, 31] MGGA functional

predicts lattice constants that are slightly smaller than those of PBE, but with

improvement in bulk moduli being rather limited. The revised TPSS (revTPSS) [32,33]

alleviates the lattice-constant error, but both TPSS and revTPSS worsen cohesive

energies compared to PBE. [13, 17] Comparing existing literature benchmarks for the

performance of LDA, PBE, PBEsol, and TPSS/revTPSS (see table 1), we see that none

of these functionals is able to describe all cohesive properties with high accuracy.

Recently, Sun, Ruzsinszky and Perdew [34] proposed the “strongly constrained and

appropriately normed” (SCAN) meta-GGA. This functional represents a major step in

the non-empirical or constraint-based construction of semi-local approximations, as it is

the first meta-GGA functional to satisfy all 17 known exact constraints that a meta-GGA

can fulfill. Appropriate norms were also added to ensure the functional is accurate for

the energies of rare-gas atoms and nonbonded interactions. SCAN has been evaluated for

properties of diversely bonded systems, including standard molecular test sets, layered

materials, and surface-adsorbate systems. [34–38] It has been shown that SCAN can

predict accurate structures and energies for the G3, BH76, and S22 sets. [34–36] In many

cases, SCAN yields improvements over other (semi-)local functionals and could be as

accurate as a fully nonlocal hybrid functional with decreased computational cost. [37,38]

Table 1. The mean absolute error (MAE) in lattice constants a0 (A), cohesive energies

E0 (eV/atom), and bulk moduli B0 (GPa) on testing sets of bulk crystals using different

density-functional approximations reported from literature benchmarksa. The mean

absolute relative error (MARE) and the maximum absolute relative error (MAX) are

given in percentage.

LDA PBE PBEsol TPSS revTPSS HSE06

a0 MAE 0.071 0.061 0.030 0.054 0.039 0.033

MARE 1.5 1.2 0.6 1.1 0.8 0.7

MAX 4.9 2.8 2.3 4.1 3.3 2.0

B0 MAE 11.5 12.2 7.8 9.6 9.6 7.3

MARE 9.4 11.0 7.0 10.3 9.4 4.0

MAX 32.8 25.5 19.5 29.6 25.8 23.4

E0 MAE 0.77 0.19 0.31 0.20 0.22 0.25

MARE 17.2 5.0 6.9 4.9 5.1 6.5

MAX 38.7 21.0 22.8 15.3 17.7 25.0

a The LDA, PBE, PBEsol, TPSS, and revTPSS data are taken from Ref. [19] (44

solids), and the HSE06 data are from Ref. [14] (30 solids).

Performance of various density-functional approximations for cohesive properties of 64 bulk solids4

The weaknesses or deficiencies in current local and semi-local DFAs are often

explained in terms of two effects: the presence of self-interaction errors and the lack

of long-range van der Waals (vdW) interactions. [3–6] As a result, the fourth and fifth

rungs of Jacob’s ladder specifically target these effects with hybrid functionals and the

random-phase approximation (RPA), respectively. Hybrid functionals add a fraction

of exact exchange to conventional GGAs or MGGAs, with the aim of reducing self-

interaction errors. [39,40] With the use of range separation of the exchange interaction,

hybrid functionals have become particularly popular in solid-state physics. HSE06

[41, 42] is among the most-widely used screened hybrid functionals, and often shows

superior performance over LDA, GGAs, and MGGAs in describing some bulk properties,

including lattice constants and band gaps. [43–51] However, both bulk moduli and

cohesive energies can be worse than those of PBE. [14] On the other hand, there is

a considerable growth of computational cost with the system size N (the number of

electrons or basis functions) using a hybrid functional compared to GGAs or MGGAs

(sometimes up to 100 times higher [52]). Thus it is often advantageous to use a GGA

or a MGGA functional for studies in condensed-matter physics and materials science.

On the fifth rung of Jacob’s ladder, the RPA is an approach that treats long-range

correlation seamlessly. Recent calculations performed by Harl et al. [53] show that

the RPA provides a well-balanced prediction of lattice constants and bulk moduli for

a diverse range of solids (including semiconductors, ionic crystals, and metals), with

relative accuracy of 0.4% and 4%, respectively. However, there are also challenges when

using the RPA. Performing self-consistent RPA is computationally very demanding, and

therefore most practical RPA calculations are performed in a post-processing manner

based on an LDA or GGA reference calculation, with the starting point being crucial

for some systems. [54,55] Furthermore, when the RPA does not start from Hatree-Fock

orbitals, there is also a first-order contribution that arises from single excitations, [56]

which often is omitted.

Given the current performance of DFAs for predicting cohesive properties, it is clear

that there is much to be done in developing new functionals. However, the deviations

themselves can be useful in this, as they are not random and clear systematic trends

can be observed for many systems. For example, Grabowski and co-authors [57] have

shown a correlation between the deviations from experiment of the lattice constants and

the bulk moduli for nine fcc metals (noble metals, together with Al and Pb), with an

increase of the error with the number of d electrons among the 4d and 5d transition

metals particularly apparent for PBE.

Analysis of wider trends may point to systematic failures for specific DFAs for

specific classes of solids, suggesting approaches to improve functionals and providing

new insights in the cohesion of solids. This makes accurate benchmarking of DFAs

and exploration of trends in deviations for a large set of solids paramount. In this

work, calculations of cohesive properties are reported on the first four rungs of Jacob’s

ladder for 64 crystalline solids. We focus on assessing the performance of six functionals,

particularly from the perspective of examining trends in performance of the different

Performance of various density-functional approximations for cohesive properties of 64 bulk solids5

functionals for different classes of solids and the relationships between the deviations in

different properties. Particular attention has been paid to convergence of the results, as

well as to understanding the different contributions not only to calculated results but

also to experimental quantities. All experimental cohesive properties will include some

contribution due to vibrational motion, even at 0 K, while the inclusion of zero-point

energy (ZPE) has long been considered in computational studies. [58, 59] Thus, any

careful comparison of theory and experiment must consider ZPE to ensure a fair and

unbiased comparison.

In the present study, the first two rungs are represented by LDA, and PBE and

PBEsol, respectively. For the third rung we choose two MGGA functionals: M06-L and

SCAN. The M06-L functional [60] was designed to incorporate the spin kinetic-energy

density in the XC functional in an empirical way, and has been reported to outperform

other semi-local functionals for a combination of thermochemistry, thermochemical

kinetics, non-covalent interactions, bond lengths, and vibrational frequencies. [60–62]

The present study will provide a benchmark of M06-L for a wide range of solids, including

solids of heavier elements, with which the functional has not been widely studied. As

noted above, SCAN represents a significant improvement over PBE (and even more so

over LDA) when considering different types of bonding in molecules [34, 38], but to-

date there has been relatively little benchmarking of it for such a wide range of hard

solids. Tran et al. [19] have calculated the lattice constants, cohesive energies, and bulk

moduli of 44 solids within the SCAN functional. We are extending the benchmark with

our larger dataset and the comparison is shown in the supplementary material. On

the fourth rung of Jacob’s ladder, we employ the HSE06 functional. Finally, we use

the screened Tkatchenko-Scheffler vdW approach to discuss the role of long-range vdW

interactions in the cohesive properties of solids.

The following section (section 2) provides details of the calculations, including the

database of solids, computational parameters and the approaches to calculating vdW

interactions and ZPE. Section 3 presents the results and discussion, including the general

performance of each functional for the solids, a discussion about trends in performance

and deviations of cohesive properties, and the role of vdW interactions.

2. Technical Details

2.1. Solid dataset

Our dataset comprises 64 crystalline solids with cubic structures: 24 metals and 40

semiconducting and insulating solids. The structures cover: A1 (face-centered cubic,

13 solids), A2 (body-centered cubic, 11 solids), A4 (diamond, four solids), B1 (rock-

salt, 16 solids), and B3 (zincblende, 20 solids), as shown in figure 1. To explore and

understand trends, we divide these 64 solids into five classes, as follows (see table 2):

main-group metals (MM), transition metals (TM), semiconductors (SC), ionic crystals

(IC), and transition-metal carbides and nitrides (TMCN). MM includes groups IA and

Performance of various density-functional approximations for cohesive properties of 64 bulk solids6

IIA, together with aluminum and lead; TM covers periods 4–7 of the periodic table;

SC represents the solids of groups IVA, IIIA–VA, and IIB–VIA; the six ionic crystals

are LiCl, LiF, NaCl, NaF, MgO, and MgS; and there are 10 compounds in the TMCN

class (TMC and TMN, TM = Ti, Zr, Hf, V, and Nb). The full list of the solids studied

here is shown in the supplementary material, [63] with the calculated and experimental

cohesive data tabulated in tables SII to SVII, alongside the relevant literature.

2.2. DFT total energy calculations

All calculations were performed employing the FHI-aims package, [64] which implements

full-potential, all-electron electronic-structure theory with numeric atom-centered

orbital basis functions. These basis functions are grouped together as “tiers” (levels) in

FHI-aims in addition to a minimal basis of occupied orbitals of spherically symmetric

free atoms. Besides, there are different sets of numerical defaults for each atomic

species, namely light, tight, and really tight settings. [64] For numerical accuracy and

computational efficiency purposes, tight setting with tier 2 basis sets are recommended

for obtaining cohesive properties of bulk solids, [20] and are employed throughout this

work. The typical tight setting convergence criteria are 10−5 electrons for the electron

density, 10−3 eV for the eigenvalues, and 10−6 eV for the total energy of the system. A

meV level of convergence is achieved for the cohesive energy.

For each solid, the equilibrium volume V0 and bulk modulus B0 were determined

by fitting cohesive energies per unit cell at 7–11 different points in a range of V0 ± 20%

to a third-order Birch-Murnaghan equation of state (EOS) [65]

E(V ) = E0+9V0B0

16

(V0

V

) 23

− 1

3

B′0 +

(V0V

) 23

− 1

26− 4(V0V

) 23

,(1)

where V0, E0, B0, and B′ correspond to the equilibrium unit-cell volume, the cohesive

energy, the bulk modulus at V0, and the pressure derivative of the bulk modulus,

respectively. The unit-cell volumes V are related to the lattice constants a by the

expressions V = a3/4 for the face-centered cubic (fcc), diamond, and zincblende

structures, and V = a3/2 for the body-centered cubic (bcc) structure. The cohesive

energy, defined as the energy per atom required to atomize the crystal, was evaluated

using the LDA, PBE, PBEsol, SCAN, M06-L, and HSE06 functionals from the energies

of the crystal and the constituent free atoms. Note that both SCAN and M06-L

calculations were performed using the PBE orbitals, as the functionality to perform

calculations with these functionals in self-consistent manner is not yet available within

FHI-aims. For SCAN, the effect of non-self-consistency has been assessed by Tran et

al., [19] and they suggest the difference between self-consistent and non-self-consistent

calculations of hard solids should be in most cases below 0.005 A for the lattice constant

and 50 meV/atom for the cohesive energy (see supplementary material).

The spin-restricted formalism was employed for bulk crystals, with two exceptions

(the ferromagnetic metals: Fe and Ni), and the spin-unrestricted formalism for open-

Performance of various density-functional approximations for cohesive properties of 64 bulk solids7

Figure 1. The unit-cell structures of (a) A1-fcc, (b) A2-bcc, (c) A4-diamond, (d)

B1-rock-salt, and (e) B3-zincblende.

shell atoms (no fractional occupancies were allowed). The basis sets and k-point meshes

in reciprocal space are fully converged. Here we used Γ-centered Monkhorst-Pack [66] k -

grids, and the settings for most calculations are outlined in the supplementary material.

Relativistic effects are more important for heavy elements; here for consistency a

scalar-relativistic treatment using the scaled zero-order regular approximation [67] was

employed for all solids. It should be noted that spin-orbit coupling, which can be

important in heavy solids, is not included. However, Philipsen and Baerends [68]

have compared the scalar-relativistic and fully relativistic calculations of the cohesive

properties of 11 solids in four columns of the periodic table and determined that spin-

orbit coupling effects barely altered lattice constants, cohesive energies, and bulk moduli,

with mean absolute contributions of about 0.005 A, 0.03 eV, and 1 GPa, respectively.

They showed that the spin-orbit coupling contributions were only non-negligible for the

cohesive energies and the lattice constants of Au and Bi. Therefore, the scalar-relativistic

treatment is sufficient to capture the relativistic effects in the solids considered here.

Table 2. The present dataset consists of five classes of solids: main-group

metals (MM), transition metals (TM), semiconductors (SC), transition metal carbides

and nitrides (TMCN), and ionic crystals (IC).

Type of solid Type of structure Number of solids

MM A1, A2 9

TM A1, A2 15

SC A4, B3 24

IC B1 6

TMCN B1 10

Performance of various density-functional approximations for cohesive properties of 64 bulk solids8

2.3. Inclusion of the long-range screened van der Waals interactions in DFT

vdW interactions arise from the correlated motion of electrons and constitute a large

part of the long-range electron correlation energy. While most commonly used DFAs

lack the ability to describe the long-range correlation energy, they provide a route to

the inclusion of the vdW energy in an effective way. Numerous promising ideas have

been proposed for including the vdW energy in DFT motivated by the need to treat

large and complex molecular and condensed-matter systems. [69–72]

One of the most widespread approaches is the pairwise-additive fragment-based

one. According to second-order pertubation theory, the vdW energy of a collection of

fragments (atoms or molecules) can be expressed as sum of attractive contributions,

with the leading nonvanishing term being due to dipole-dipole interactions

EvdW = −1

2

∑i

∑j

fdampCij

6

R6ij

, (2)

where Rij is the interatomic distance between atoms i and j of the system, Cij6 is

the corresponding dipole-dipole dispersion coefficient, and fdamp is a damping function

that is used to avoid singularities at short distances and ameliorate double-counting

of correlation at intermediate distances. [69–72] The resulting vdW energy is then

augmented to the standard KS-DFT total energy calculated by employing a local, semi-

local or hybrid DFAs. In principle, the accuracy of any fragment-based DFT-vdW

method, referred to as “DFT+vdW” here, depends solely on the coefficients used and

the choice of the damping function.

The leading-order C6 term can be expressed as

Cij6 =

3

π

∫ ∞0

αi(iω)αj(iω)dω, (3)

where the integrand contains the isotropic dipolar polarizability as a function of

imaginary frequency. Thus the polarizablity is a central quantity to the description

of vdW interactions. The method employed here is based upon the Tkatchenko-

Scheffler (TS) scheme, [73] which computes the polarizability, the C6 dispersion

coefficient and the vdW energy by ultilizing Hirshfeld partitioning [74] of the electron

density to rescale free-atom values [75] obtained from self-interaction corrected time-

dependent DFT calculations. The TS approach yields accurate C6 coefficients for a

set of 1225 small molecules (with an accuracy of 5.5%) due to its ability to capture

local enviromental effects. However, TS lacks the ability to describe the long-range

electrostatic screening that extends beyond the range of the exponentially decaying

atomic densities. These effects can be included microscopically by modeling the

environment as a dipole field of quantum harmonic oscillators (QHOs) and solving the

resulting classical electrodynamics self-consistent screening (SCS) equation. [76]

In this model, a molecule (or material) is considered as an arrangement of N atoms,

each of which is described by a spherical QHO. [72, 76, 77] For a given atom i in the

Performance of various density-functional approximations for cohesive properties of 64 bulk solids9

system, one can write

αSCSi (r , iω) = αTS

i (r , iω) + αTSi (r , iω)

N∑i 6=j

TijαSCSj (r ′, iω), (4)

where αSCSi (r , iω) is the fully screened atomic polarizability tensor (for a given frequency

of the electric field), containing both short-range (via the input atomic polarizability

tensor from the TS method) and long-range (via the SCS equation) screening effects.

The dipole-dipole interaction tensor, Tij, has the following expression

Tij = ∇r i⊗∇r j

V (rij), (5)

where V (rij) is the Coulomb potential between two spherical Gaussian distributions at

the distance rij, with r i and r j representing the QHO positions. The solution of the SCS

equation yields the atomic polarizability tensors, from which the isotropic polarizability

can be obtained by diagonalizing and tracing the tensor. To calculate the C6 dispersion

coefficient (via equation 3), the Gauss-Legendre approach is utilized. [76]

In this work, we calculate dipolar polarizabilities and C6 dispersion coefficients for a

set of 23 semiconductor solids using the method introduced above, and use them via the

DFT+vdW scheme to evaluate the role of vdW interactions in the cohesive properties

of solids.

2.4. Calculation of zero-point vibrational energy

Zero-point vibrational energy effects have been evaluated using the quasi-harmonic

approximation. Phonon calculations were performed using phonopy [78] interfaced

with the FHI-aims package. [79] The supercell approach [80] was combined with the

quasi-harmonic approximation, i.e., for a set of different volumes, harmonic vibrational

frequencies are determined using ab initio calculations, with the zero-point energies

being added to the DFT ground-state energies at each volume V. In the FHI-aims

package, the finite-displacement method is employed to calculate phonon spectra and

the vibrational density of states (DOS), g(V, ω), and ZPE is estimated as the frequency

integration over the vibrational DOS

ZPE =1

2

∫hωg(V , ω)dω. (6)

A systematic test of the supercell size was carried out and it was found that a

choice of a 2 × 2 × 2 supercell with a 8 × 8 × 8 k-point grid is sufficient to ensure the

convergence of zero-point vibrational energies for all the solids studied here. Within the

finite-displacement approach, one may adjust the value of the small finite displacement

δ used to calculate the force response in the three Cartesian directions. This has also

been systematically tested, demonstrating that a reasonable variation in δ has only

a small impact on the computed ZPE. For example, the ZPE for diamond is about

0.18 eV/atom, and the change in ZPE is less than 1 meV/atom (0.2%) when varying

δ from 1 × 10−3 to 1 × 10−1 A. In addition, it was found that the effect of the specific

DFT functional on the ZPE is negligible for these systems, and as a result, ZPE was

Performance of various density-functional approximations for cohesive properties of 64 bulk solids10

calculated at the PBE level and added on top of the ground-state DFT total energies

for all six functionals.

For the analysis of our calculations, we consider statistical quantities: the mean

error (ME), the mean absolute error (MAE), the mean relative error (MRE, %), and

the mean absolute relative error (MARE, %), all of which are determined by comparing

with reliable experimental values measured at low temperatures and/or extrapolated to

0 K.

3. Results and discussion

3.1. ZPE contributions to the cohesive properties

We start by discussing the contribution of ZPE to the cohesive properties of the solids

in our dataset. Figures 2 and 3 show the relative contributions of ZPE to the lattice

constants a0, the cohesive energies E0, and the bulk moduli B0 of selected metals and

non-metallic solids, respectively, together with available theoretical values reported from

previous work. [12,14,81] A summary is given in table 3 for all of the solids considered

in the present work. The results show that including zero-point vibrations has an even

stronger effect on the bulk modulus than on both the lattice constant and the cohesive

energy. For 24 metals, the average contributions are 0.2%, 0.7%, and 1.4% for a0, E0,

and B0, respectively. In addition, the ZPE effect is, as expected, inversely proportional

to nuclear mass (e.g., along the series of Li-Na-Al-K), and is found to be negligible for

“heavy” solids. When only considering the “light” metals, located on the second to

fourth rows of the periodic table, the averaged contribution is almost twice as large as

the value calculated for the whole group of metals. In particular, for bulk Li, the lattice

constant expands by 0.7% and the bulk modulus reduces considerably by ∼4%.

For non-metallic solids, ZPE contributions become more pronounced. A set of 40

solids shows average contributions of 0.3% to the lattice constants, 1.1% to the cohesive

energies, and 2.2% to the bulk moduli. For ionic crystals, the effect is particularly

strong. The largest contribution occurs for LiF, with changes of about 1% (0.04 A)

for a0 and 8% (5.6 GPa) for B0, which are much larger than numerical errors in DFT

calculations, and even might be comparable to the contribution due to the long-range

electron correlation. [82] This suggests that for non-metallic solids, especially ionic

crystals, the inclusion of ZPE becomes vital for an accurate assessment of systems

where long-range vdW interactions can be of relevance.

In comparison with existing literature data, our results are in excellent agreement

with the calculations reported by Schimka and co-authors [14] using the projector

augmented wave method implemented in the Vienna Ab Initio Simulation Package [83,

84]. Their dataset comprises 30 solids (including seven metals, six ionic crystals, and

Performance of various density-functional approximations for cohesive properties of 64 bulk solids11

Table 3. Zero-point vibrational contributions to the lattice constants a0 (A), cohesive

energies E0 (eV/atom), and bulk moduli B0 (GPa) of 64 solids (24 metals, 40 non-

metals, including six ionic crystals). The values in parentheses are the corresponding

percentage with respect to the reported experimental cohesive properties (%). The 24

metals are divided into two groups: nine elements from periods 2–4, and 15 elements

from periods 5–7 of the periodic table.

a0 E0 B0

All metals 0.007 0.023 1.5

(0.2) (0.7) (1.4)

Periods 2-4 0.011 0.029 1.7

(0.3) (1.1) (2.1)

Periods 5-7 0.004 0.020 1.4

(0.1) (0.5) (0.9)

Non-metals 0.012 0.054 3.4

(0.2) (1.1) (2.2)

Ionic crystals 0.026 0.044 2.9

(0.6) (1.1) (4.4)

17 semiconductors). For some metals (like Li, Rh, and Cu) and most non-metallic

solids, their corrections to both the lattice constants and cohesive energies are essentially

identical to the present results, as shown in figures 2 and 3. To the best of our knowledge

the evaluation of the ZPE contribution to the bulk moduli has not been performed

previously for such a diverse set of bulk solids.

The present study confirms that ZPE tends to increase lattice constants and reduce

bulk moduli, with its inclusion improving the predictions of the LDA functional and

worsening those of PBE (cf. table 1). As a result, neglecting zero-point vibrations will

lead to a bias in the appraisal of these and other DFAs. Therefore, in the following

sections, ZPE vibrational contributions will always be included in the discussion of

functional performance.

3.2. Performance of density functionals along Jacob’s ladder

Having assessed the impact of ZPE, we can now study the performance of local,

semi-local, and hybrid DFAs for the dataset of 64 solids. The calculated a0, E0, and B0

using the LDA, PBE, PBEsol, SCAN, M06-L, and HSE06 functionals are tabulated in

tables SII to SVII of the supplementary material [63], together with their experimental

values, while the mean relative and mean absolute errors are shown in table 4. To

illustrate the performance of the six functionals for different types of solids, we also plot

the relative errors in the bulk moduli and the cohesive energies as a function of those in

the lattice constants for the specific groups of solids in figures 4 and 5, respectively. The

Performance of various density-functional approximations for cohesive properties of 64 bulk solids12

0

0.5

1

1.5

a0 (

%)

0

1

2

3

E0 (

%)

02468

B0 (

%)

NaLi

NiKCa

VFeAl Cu Sr Mo

RhPd

AgBa

TaW

IrPt Pb

Au ThRb Nb

Figure 2. Zero-point vibrational contributions to the lattice constants a0, cohesive

energies E0, and bulk moduli B0 of selected metals. The values are shown as a

percentage with respect to the experimental cohesive properties, with the solid curves

representing the present ab initio phonon calculations, pink pluses are taken from

Ref. [81], and green crosses from Ref. [12].

0

0.5

1

1.5

a0 (

%)

0

1

2

3

E0(%

)

02468

B0 (

%)

LiClLiF

BAsNaCl BNMgO BPNaF

GaAsC Si

SiC GeSn

AlPAlAs

GaNGaP

InAsInP InSb

Figure 3. Zero-point vibrational contributions to the lattice constants a0, cohesive

energies E0, and bulk moduli B0 of selected non-metallic solids. The solid lines are

obtained from the present ab initio phonon calculations, green crosses are taken from

Ref. [12], and purple stars are from Ref. [14].

corresponding MAREs are presented in table 5 in terms of classes of solids, properties,

as well as functionals.

Let us first discuss the performance of the LDA functional. The present work

confirms the well-known trend that LDA underestimates lattice constants, overestimates

bulk moduli, and considerably overestimates cohesive energies in most situations. From

the MAREs of the three properties summarized in table 5, one can clearly observe

Performance of various density-functional approximations for cohesive properties of 64 bulk solids13

that LDA shows a different performance for the different classes of solids. For the SC

class, it predicts the lattice constants and the bulk moduli in good agreement with

experiment, however at the expense of the cohesive energies, while for ionic crystals

it yields moderately accurate results. However, for metals (groups MM and TM) the

performance of LDA is unsatisfactory. Note that the performance of LDA for 4d and

5d transition metals is better than 3d and main-group metals.

Turning to the PBE functional, one can see the opposite trend to LDA: Lattice

constants are too large, and the bulk moduli are too small. Cohesive energies are

significantly improved though, with a MARE of ∼6% versus ∼20% for LDA for the

64 solids. Overall, PBE improves the agreement with experiment compared to the

LDA functional. For the MM and 3d metals, the superiority of PBE over LDA for

calculating cohesive properties becomes particularly prominent. For semiconductors

and ionic crystals, PBE yields large deviations from experimental results for both the

lattice constants and the bulk moduli, while the cohesive energies are reasonably well

predicted. A characteristic feature of the PBE functional observed in the current study

is the increase of the error with increasing lattice constant, as can be seen, e.g., along

the series of C-SiC-Si-Ge-Sn, BN-BP-BAs, and AlP-AlAs-AlSb. For certain systems,

the bulk moduli and the cohesive energies follow the same trend. We will return to

this observation in section 3.3, when exploring the underlying causes for deviations and

trends in the DFAs considered here.

The PBEsol functional was first proposed to improve the description of solids and

surfaces compared to PBE. [25] For lattice constants, it does indeed yield improvements,

curing the problem of underbinding. In fact, it slightly overbinds bulk crystals. The

current study shows significant improvement in the lattice constants using PBEsol

for semiconductors, insulators, and fcc metals (except the alkaline-earth elements, Ni,

Cu, and Th). Consistently, the bulk moduli are much better predicted with PBEsol

compared to PBE for the aforementioned systems. For instance, the MAREs are 0.4%

and 0.5% respectively for the lattice constants of the SC and IC classes by PBEsol

(versus 1.6% and 1.8% by PBE). The corresponding MAREs for the bulk moduli are

very similar for the same solids, both about 6% (versus 14.5% and 16%, respectively, by

PBE). For the rest of the solids, i.e., the bcc metals (except K and Rb) and TMCN, both

lattice constants and bulk moduli calculated with PBEsol are only marginally better or

even worse than with PBE. This agrees with the finding by Janthon and co-authors [85]

in a study of 30 transition metals. The substantial change from PBE to PBEsol is

a consistent shift of the bonding nature towards tightening: decreasing of the bond

lengths (lattice constants) and increasing of the bulk moduli. Overall, PBEsol shows

overbinding of solids. One “expected” problem of using the PBEsol functional, which

is observed in the present data, is that the calculated cohesive energies are inaccurate,

only halving the LDA error and twice as large as the PBE ones. This can be traced

back to inaccurate total energies of the individual atoms. [25]

Turning to the meta-GGA functionals, the overall performance of M06-L for

cohesive properties lies between that of LDA and PBE. However, no consistent trend

Performance of various density-functional approximations for cohesive properties of 64 bulk solids14

Table 4. The mean error (ME) and mean absolute error (MAE) in the calculated

lattice constants a0 (A), cohesive energies E0 (eV/atom), and bulk moduli B0 (GPa)

of the 64 solids using the LDA, PBE, PBEsol, SCAN, M06-L, and HSE06 density

functionals, with respect to experimental values. The mean relative error (MRE, %)

and mean absolute relative error (MARE, %) are given in parentheses. The maximum

absolute relative error (MAX, %) is shown in the last columns, within the solid marked

in boldface using each functional. All quantities include zero-point vibrational effects.

Functional ME MAE MAX

a0 E0 B0 a0 E0 B0 a0 E0 B0

LDA −0.063 0.85 13.0 0.063 0.85 15.4 4.9 48.4 46.0

(−1.4) (19.3) (8.2) (1.4) (19.3) (10.6) Ba Fe Fe

PBE 0.056 −0.08 −9.8 0.061 0.21 13.6 2.8 19.4 33.2

(1.1) (−2.1) (−9.6) (1.2) (5.5) (11.6) Pb Au Sn

PBEsol −0.010 0.37 3.5 0.030 0.39 10.7 2.9 31.5 32.7

(−0.3) (8.2) (−0.5) (0.6) (8.9) (7.4) Th Fe Fe

SCAN 0.011 −0.08 4.1 0.028 0.23 9.0 2.7 17.4 26.1

(0.1) (−0.7) (0.7) (0.6) (5.4) (5.9) Th Mo V

M06-L 0.031 0.18 −4.3 0.075 0.27 12.2 6.1 52.8 61.3

(0.5) (6.8) (−2.4) (1.4) (9.0) (13.1) Rb Rb Rb

HSE06 0.036 −0.37 1.6 0.042 0.40 12.2 3.2 32.6 35.0

(0.7) (−7.5) (−2.5) (0.8) (9.1) (8.6) Rb V V

can be identified. The current work suggests that M06-L significantly improves the

performance on the cohesive properties of ionic crystals in comparison with LDA,

GGAs, and hybrid functionals. For the six solids, it slightly overestimates the lattice

constants, and reasonably predicts the cohesive energies and the bulk moduli, with

resulting MAREs of 0.3%, 3.3%, and 4.9%, respectively. On the other hand, for most

semiconductors, M06-L overestimates lattice constants, and underestimates cohesive

energies, as well as the bulk moduli. In particular, for main-group metals, M06-L

severely overbinds: the lattice constants are too small, and both the cohesive energies

and the bulk moduli are too large. For transition metals, M06-L improves the lattice

constants of 3d elements in better agreement with experiment, but worsens the other two

properties; a significant improvement in cohesive energies is found only for the coinage

metals (Pd, Pt, Ag, and Au), however at the expense of both the lattice constants and

the bulk moduli. Overall, the M06-L functional performs less accurately than PBE for

the TM group, as can be seen from table 5.

The recent SCAN functional is a non-empirical meta-GGA, unlike M06-L, and is

the first functional to fulfil all known constraints that a meta-GGA can fulfil. The

current study reveals that SCAN predicts remarkably accurate cohesive properties for

a diverse set of bulk crystals and tends to strike a good balance between PBE and

PBEsol. For non-metallic systems, significant and consistent improvement is found for

Performance of various density-functional approximations for cohesive properties of 64 bulk solids15

the predictions of all three cohesive properties using the SCAN functional: the lattice

constants are very accurate, with a MARE of less than 0.5% for each class of solids,

while both the bulk moduli and the cohesive energies are reasonably well predicted. Our

work also suggests that particularly for ionic and semiconductor solids, SCAN remains

the best method of choice among the six density functionals tested here, with MAREs

within 0.5%, 3%, and 5% for a0, E0, and B0, respectively. For the MM group, SCAN

performs equally as well as PBE does for the prediction of the lattice constants, but

yields a better prediction of bulk moduli, while for the TM group, the performance

of SCAN is as good as PBEsol. Overall, SCAN overestimates the bulk moduli of the

bcc metals and underestimates those of the fcc metals. Especially for the 4d and 5d

coinage metals (Pd, Ag, Pt, and Au), SCAN cures the underbinding problem of PBE

to a large extent. To our knowledge, a theoretical assessment on the reliability of the

SCAN functional was first performed by the SCAN authors themselves, [34] for the

lattice constants of 20 solids. To compare the present results to their data, we consider

the same set of 20 solids. The mean absolute deviation and mean deviation of the lattice

constants are calculated to be 0.01 A and 0.002 A respectively between the two studies.

This suggests our post-SCF procedure is a good approximation for the current work.

A further evaluation of SCAN for other cohesive properties should be performed in the

future.

The final DFA tested in the present work is the HSE06 hybrid functional. HSE06

predicts reliable lattice constants and bulk moduli for non-metallic crystals and its

performance is only slightly worse than SCAN and PBEsol. For both the ionic and

semiconductor solids, the general trend that HSE06 overestimates the lattice constants,

underestimates the bulk moduli, and predicts reasonably good cohesive energies is

confirmed. While HSE06 improves agreement with experiment for the lattice constants

of TMCN, it underestimates the cohesive energies, and considerably overestimates the

bulk moduli. Our study indicates that HSE06 exhibits an overall tendency to underbind

solids, and this can be pronounced for metals. The overestimation of the lattice

constants is found for nearly all of the metals (with the exception of V). Especially

for the main-group metals (except Al and Pb), the HSE06 lattice constants are even

larger than the PBE values, with a corresponding decrease in bulk moduli. For the TM

group, a large difference is seen between the fcc and bcc metals: HSE06 overestimates the

bulk moduli for nearly all bcc-TM (except for Fe), whereas it typically underestimates

those for fcc-TM (except for Rh). In addition, the cohesive energies show significantly

increased errors compared to the PBE results. This can be explained by the fact

that hybrid functionals generally increase the stability of the spin-polarized atom, thus

reducing stability of bulk systems. [48,49]

Figures 4 and 5 show comparisons of the density functionals tested here for

describing the cohesive properties of all five classes of solids. Among the six functionals,

LDA predicts accurate lattice constants and bulk moduli for semiconductors, however,

the cohesive energy remains a considerable issue at this level, with a MARE of ∼20%

for the 24 solids in this group. While PBE outperforms LDA on the prediction of

Performance of various density-functional approximations for cohesive properties of 64 bulk solids16

Table 5. The mean absolute relative error (MARE, %) for the lattice constants a0,

cohesive energies E0, and bulk moduli B0 of the 64 solids divided into five classes (see

main text for definitions).

LDA PBE PBEsol SCAN M06-L HSE06

a0 MM 3.1 0.9 1.0 0.9 3.1 1.2

TM 1.6 1.1 0.9 0.8 1.6 0.9

SC 0.6 1.6 0.4 0.5 1.7 0.8

IC 1.5 1.8 0.5 0.2 0.3 0.8

TMCN 1.2 0.5 0.5 0.3 0.6 0.4

E0 MM 20.4 8.5 13.7 12.4 37.1 11.2

TM 25.1 6.5 12.5 7.4 8.3 16.8

SC 19.3 5.0 7.6 2.4 2.6 4.6

IC 8.1 5.1 1.4 1.7 3.3 6.0

TMCN 15.9 2.6 6.9 5.6 3.7 7.6

B0 MM 12.1 7.0 4.5 4.4 30.5 8.3

TM 17.5 8.9 9.3 8.0 10.1 11.2

SC 4.6 16.0 6.3 4.4 13.2 5.9

IC 9.0 14.5 6.4 3.8 4.9 7.0

TMCN 13.9 7.5 10.1 8.8 7.5 12.6

the cohesive energies for semiconductors, it worsens both the lattice constants and the

bulk moduli. In fact, the improved performance of PBE upon LDA can be mainly

seen in its better description of the cohesion in the systems having a (semi-)metallic

nature. As depicted in figures 4 and 5, all the cohesive properties obtained using

PBE are in much better agreement with experiment for the MM, TM and TMCN

groups, compared to the LDA results. Among the six functionals, PBE remains the best

for the 3d transition metals. The PBEsol functional cures the underbinding of PBE,

however it somewhat overbinds, but yields reliable lattice constants and bulk moduli

for ionic crystals, semiconductors, and fcc metals. Employing PBEsol, the MARE of

semiconductors is reduced by a factor of four for lattice constants and two and a half

for bulk moduli respectively, compared to the PBE errors. Overall, the PBEsol cohesive

energies show systematic overestimation, halving the LDA deviation, with the exception

of ionic crystals for which PBEsol yields accurate predictions. The HSE06 functional

corrects the lattice constants, and improves agreement with experiment for ionic and

semiconductor solids, however it still shows a tendency to underbind. The increased

errors in cohesive energies, together with the demanding computational cost, remain

significant issues for using the HSE06 functional.

In comparison, the M06-L MGGA functional improves on LDA for TM and TMCN

(though its performance is slightly worse than PBE), however it yields significant

deviations from experiment for the main-group metals, as seen in table 5. This is

Performance of various density-functional approximations for cohesive properties of 64 bulk solids17

−40

−30

−20

−10

0

10

20

30

40

−6 −4 −2 0 2 4 6

LDAPBE

PBEsolSCAN

M06−LHSE06

−80

−60

−40

−20

0

20

40

60

80

−6 −4 −2 0 2 4 6

−40

−30

−20

−10

0

10

20

30

40

−6 −4 −2 0 2 4 6

−40

−30

−20

−10

0

10

20

30

40

−6 −4 −2 0 2 4 6

SC TMCN

ICMM,TM

Deviation of a0 from experiment (%)

Dev

iati

on

of

B0 f

rom

exp

erim

ent

(%)

Figure 4. Correlation between the deviations of the bulk moduli B0 (%) and those of

the lattice constants a0 (%) using the LDA, PBE, PBEsol, SCAN, M06-L, and HSE06

functionals. The definitions of the five classes of solids are given as main-group metals

(MM), transition metals (TM), semiconductors (SC), transition metal carbides and

nitrides (TMCN), and ionic crystals (IC). All quantities include zero-point vibrational

effects.

consistent with the study by Zhao and Truhlar. [61] Compared to PBE, M06-L performs

better for semiconductors with lighter elements. For C, Si, BN, BP, and AlP, the

cohesive properties obtained from M06-L are in good agreement with experiment. The

bulk moduli calculated with M06-L are as good as the LDA values, whereas PBE yields

the worst performance among the six functionals, while the M06-L cohesive energies

are greatly improved compared to the LDA results. However, when considering heavy-

element systems, there is barely any improvement to be gained by using M06-L over

PBE. This can be seen for the cases of GaSb, InSb, ZnTe, CdTe, etc. Similar behaviour

is also observed for ionic crystals. The M06-L functional significantly improves the

description for the six ionic compounds that have medium mass, with a MARE of

only 0.3% for the lattice constants versus those of 1.5% and 1.9% by LDA and PBE,

respectively. Turning to the non-empirical MGGA functional, our study suggests that

SCAN can be regarded as the method of choice for non-metallic solids and it agrees

remarkably well with experiment for all the three cohesive properties. The SCAN lattice

constants are considerably smaller than those of PBE, with an increase of the bulk

moduli and larger cohesive energies. For metals, no significant improvement is found

on the lattice constants and bulk moduli, while SCAN worsens the cohesive energies

Performance of various density-functional approximations for cohesive properties of 64 bulk solids18

−40

−30

−20

−10

0

10

20

30

40

−6 −4 −2 0 2 4 6

−80

−60

−40

−20

0

20

40

60

80

−6 −4 −2 0 2 4 6

−40

−30

−20

−10

0

10

20

30

40

−6 −4 −2 0 2 4 6

LDAPBE

PBEsolSCAN

M06−LHSE06

−40

−30

−20

−10

0

10

20

30

40

−6 −4 −2 0 2 4 6

SC TMCN

ICMM,TM

Deviation of a0 from experiment (%)

Sn

VNVCVN

VC

ZnTe CdTe

Pb

V

V

Th

Rb

Ni

Dev

iati

on o

f E

0 f

rom

exper

imen

t (%

)

Figure 5. Correlation between the deviations of the cohesive energies E0 (%) and

those of the lattice constants a0 (%) using the LDA, PBE, PBEsol, SCAN, M06-L,

and HSE06 functionals. Some outliers are explicitly marked.

compared to PBE. For the 4d and 5d coinage metals, SCAN substantially improves on

PBE.

In summary, our study shows that all of the functionals considered have varying

performances in predicting the cohesive properties of solids, which strongly depend on

the bonding nature of the solid. To understand these trends and behavior in more detail,

we now move to discussing the relationships between pairs of cohesive properties, that

is, a0/B0 and a0/E0.

3.3. Correlations between cohesive properties

Much attention has been paid in the literature to understanding the relationship between

geometrical parameters and properties of various classes solids and the cohesive energy

and bulk modulus. It has been found that both E0 and B0 are inversely related to a0 (or

the nearest-neighbor distance d). [86–91] This inverse relation can be explained by the

volume dependence of the total energy (the equation of state) causing a monotonic

decrease of the bulk modulus with increasing volume (cf. equation 1). There are

several analytical expressions reported in the literature for different families of cubic

solids, [86–91] e.g., semiconductors (groups IVA, IIIA–VA, and IIB–VIA), ionic crystals

(groups IIA–VIA and IA–VIIA), and metals (groups IA and IIA, and noble metals),

based upon empirical approaches. While such empirical methods are often not able to

Performance of various density-functional approximations for cohesive properties of 64 bulk solids19

yield highly accurate results, they can still be very useful, particularly for illustrating

trends in properties of a wide variety of materials.

Anderson and Nafe [86] first proposed an empirical relationship between bulk

modulus and crystal volume of the form B0 ≈ V −x0 , where x depends on the bonding

type of solid. Cohen and co-authors [87, 88] studied a number of covalent and ionic

crystals, and deduced an analytical expression between the bulk modulus and the

nearest-neighbor separation d for diamond and zincblende structures

B0d3.5 = (1971− 220λ), (7)

where λ is an empirical ionicity parameter accounting for the ionic character of the

bonds. This relationship was found to be appropriate for group IVA (λ=0), IIIA–VA

(λ=1), and IIB–VIA (λ=2). For the IA–VIIA rock-salt compounds, Cohen proposed

B0d3 = 550. (8)

A similar scaling of B0d3.5 for the rock-salt structure was suggested by Schlosser, [89,90]

and the cohesive energy was discussed in terms of d as well. Aresti et al. [91] studied

the cohesive energy of zincblende solids using the form,

E0d ≈ constant. (9)

According to the empirical expressions given by equations 7–9, an overestimation

(underestimation) of the lattice constant corresponds to an underestimation

(overestimation) of the bulk modulus or the cohesive energy. In fact, for the present

dataset all of the DFAs considered broadly follow this trend.

Figures 4 and 5 show the relative errors in the bulk moduli and the cohesive energies

as a function of the lattice-constant errors, using the LDA, PBE, PBEsol, SCAN, M06-

L, and HSE06 functionals for the 64 solids divided into five classes. It can be seen

that most data points are in the quadrants II and IV of the Cartesian plane, reflecting

that the shorter the lattice constants, the larger the bulk moduli and the cohesive

energies, and vice versa. This indicates that those DFAs can predict the observed

experimental trends (the inverse relationships of bulk moduli and cohesive energies with

lattice constants). If one further looks into the errors concerning a given type of solids,

large differences can be found for specific functionals. For SC and IC, a nearly monotonic

dependence is observed for the deviations of the bulk moduli from experiment upon

those of the lattice constants using all the functionals tested, that is, the overestimated

lattice constants is accompanied by the underestimated bulk moduli. It can also be

observed that there is a better (“linear”) correlation between the errors from the PBE

calculations, in comparison with, e.g., LDA, applied to the SC compounds, where half

of the values fall in the quadrant III, in disagreement with the empirical study based

on experimental observations. Overall, the PBE functional yields the most consistent

results with experiment, and it is the method that reproduces systematic trends in the

cohesive properties of solids better than the other functionals.

Turning to metals (the MM and TM groups), a noticeable scatter of the errors is

found, e.g., from the LDA, PBEsol, and M06-L calculations, with the inversely correlated

Performance of various density-functional approximations for cohesive properties of 64 bulk solids20

behavior being somewhat captured by the PBE, HSE06, and SCAN functionals. This

also reflects the poor performance of LDA and M06-L, particularly in the description of

main-group metals. Finally, for the TMCN group, there is no clear trend shown by any

method used here. We note that no clear experimental correlations have been found

between any pair of cohesive properties for this class of solids (see figures 6 and 7),

mainly due to the mixed nature of the metallic, covalent, and ionic bonding in these

solids. [92, 93]

-10 -8 -6 -4 -2 0Experimental E0 (eV/atom)

2

3

4

5

6

7

Exp

erim

enta

l a0(

Å)

SCTMCNMMTMIC

Al

Rb

Li

Na

K

Sr

Ca

PbBa

C

SiC

SiGe

ZrCZrN

Figure 6. The experimental lattice constant as a function of the cohesive energy for

selected semiconductors, ionic crystals and metals. The definitions of the five classes of

solids are given as main-group metals (MM), transition metals (TM), semiconductors

(SC), transition metal carbides and nitrides (TMCN), and ionic crystals (IC).

0 100 200 300 400Experimental B

0 (GPa)

2

3

4

5

6

7

Exp

erim

enta

l a0(

Å)

SCTMCNMMTMIC

LiF

NaF

LiCl

NaCl

(IA-VIIA)

MgO

(IIIA-VA, IIB-VIA)

(IVA)

Figure 7. The experimental lattice constant as a function of the bulk modulus for

selected semiconductors, ionic crystals and metals. The dashed lines serve as a guide

to the eye.

Performance of various density-functional approximations for cohesive properties of 64 bulk solids21

The above findings suggest that the errors in different cohesive properties obtained

from DFT calculations are correlated and system dependent. In general, PBE shows

superior performance to LDA, due to the inclusion of the density gradient term for

describing nonlocality in realistic systems. The improvement of PBE over LDA is

significant for main-group and 3d metals. For some semiconductors and “heavier” 4d,

5d transition metals, the cohesive properties are better predicted by LDA than by PBE

(except for the cohesive energies). When it comes to the M06-L functional, the present

study shows that it can perform well for small and medium-sized solids. This can be

ascribed to the fact that the parameters in the M06-L functional are obtained from

fits to molecular systems, allowing it to describe mid-range interactions to some extent,

which can be seen from its good performance for the ionic crystals considered here.

Furthermore, the current work suggests that investigating the relationships between

errors in cohesive properties can help us to understand performance and capability of

DFAs. In particular, it is found that the system-dependent behavior of the cohesive

properties is best reproduced at the PBE level. Indeed, by using the PBE functional

an increase of errors in bulk moduli is accompanied by that in lattice constants for

many solids in the current dataset. This is consistent with the finding by Grabowski

and co-authors, who discussed the dependence of deviations given by the LDA and

PBE functionals for fcc metals. [57] The behavior of the increasing errors with mass,

the “sizable error”, [94] can also be observed in the lattice constants. In figure 8, the

deviations of the calculated lattice constants from experiment are plotted as a function of

their experimental values for 24 metals and 40 non-metals using the six functionals. One

can see that the monotonic relationship, indicating that the systematic error increases as

the crystal unit-cell volume increases, is better reproduced by PBE and HSE06, rather

than LDA, PBEsol, M06-L or SCAN. The trend is more pronounced in non-metals than

metals, in good agreement with experiment (see figures 6 and 7). For 40 non-metallic

solids, a nearly monotonic behavior is captured using PBE, while two separate regions

are found using M06-L. Our analysis suggests the size-related error issue can be related

to the lack of the long-range electron correlation in density approximations, which is

discussed further below.

3.4. Challenges for meta-GGA and hybrid functionals

The accurate prediction of both structural and energetic properties of bulk solids remains

a difficult task for current density-functional approximations. The SCAN meta-GGA

and HSE06 hybrid functionals, which belong to the third and the fourth rungs of Jacob’s

ladder, were specifically developed to improve upon conventional LDA and GGAs. As

we have seen, semiconductors (24 solids) and insulators (six solids) benefit greatly

from SCAN and HSE06 for predicting structural properties (a0 and B0): SCAN yields

remarkably accurate lattice constants (MAREs: 0.5% and 0.2% versus 1.6% and 1.8%

by PBE), bulk moduli (MAREs: 4.4% and 3.8% versus 16% and 14.5%), while HSE06

performs reasonably well for both properties, with the errors reduced by more than a

Performance of various density-functional approximations for cohesive properties of 64 bulk solids22

−0.4

−0.2

0.0

0.2

0.4

LDA

Non−metalMetal

PBEsol

−0.4

−0.2

0.0

0.2

0.4

Dev

iati

on o

f a

0 f

rom

exper

imen

t (Å

)

PBE SCAN

−0.4

−0.2

0.0

0.2

0.4

2 3 4 5 6 7

Experimental a0 (Å)

M06−L

2 3 4 5 6 7

HSE06

SrCa

RbK

Na

LiAl

Pb

Ag,Au

SrCaTh

PbNaFLiF

SrCa

Ba

RbKNaFeV

SrCa

Ba Th

FeV

K Rb

Pb

Th

Fe V Ni Cu

K

Rb

PbAg,Au

Fe

V

Figure 8. Deviations of DFT lattice constants from experiment (A) for 24

metals (crosses) and 40 non-metals (solid squares) versus their experimental lattice

constants (A) using the LDA, PBE, PBEsol, SCAN, M06-L, and HSE06 functionals.

factor of two compared to the PBE results. The SCAN functional improves on PBE for

predicting all the three properties of semiconductor and insulator solids simultaneously

and this is clearly a substantial improvement for a semi-local DFA.

Performance of various density-functional approximations for cohesive properties of 64 bulk solids23

However, for transition metals meta and hybrid functionals generally yield no

improvement in accuracy over GGA functionals. [28, 31, 94] For the lattice constants,

PBE yields fairly accurate results for 3d metals, but systematically overestimates them

for 4d and 5d metals, consistently underestimating both bulk moduli and cohesive

energies. In particular, PBE fails to describe the cohesion in coinage metals including

Pd, Ag, Pt, and Au. The averaged errors are about 2% larger in the lattice constants,

17% in the bulk moduli, and 11% in the cohesive energies for those four metals. Note that

the size-related issue discussed in section 3.3, the increase of the error with increasing

nuclear mass, is more pronounced here. The origin of this size-related error is not fully

understood, but it is likely that this can be related to the presence of self-interaction

errors and/or the lack of the long-range electron correlation in semi-local DFAs. As vdW

interactions arise from the correlated motion of electrons, they are larger in magnitude

for larger systems (i.e., with more electrons), and constitute a significant part of the

long-range electron correlation energy. The inclusion of the attractive vdW energy helps

shorten bond lengths and stablize the crystal.

The SCAN functional (as well as M06-L) captures mid-range interactions to a

certain extent, which can be seen from its improved description for the interaction

energies of the S22 dataset. [34] When applied to solid transition metals, our results

suggest that SCAN achieves a major improvement over PBE for 4d and 5d coinage

metals where the electron correlation becomes more important between the almost filled

d shells. M06-L also performs better for medium-sized unit cells, but for those solids

with a large unit-cell volume (heavy nuclear mass), it performs worse than PBE for

cohesive properties. This is also an indication that vdW interactions are responsible for

part of the deviations of modern DFAs, with the meta-GGA form of SCAN and M06-L

allowing them to capture mid-range vdW interactions. This likely accounts for some of

the better performance of these functionals for some systems. However, the long-range

vdW interactions are still missing from these functionals, [35,36] with the present study

showing noticeable deviations from experiment for solid systems including 3d metals,

alkali and alkaline-earth metals.

Part of these deviations will also stem from self-interaction errors. [95] The HSE06

hybrid functional, partially counters self-interaction errors by admixing a fraction of

exact exchange. As already seen in section 3.2 and other studies, [48, 49] HSE06 yields

improved performance on the coheisve properties of molecules, semiconductors, and

insulators. While for metallic systems HSE06 performs worse than PBE, particularly

for the cohesive energies of transition metals, the HSE06 results deviate significantly

from experimental values, mainly due to the incorrect treatment of localized d electrons.

This illustrates both the impact of self-interaction errors and the challenge of accounting

for them. Therefore, given the different contributions that DFAs need to account for

(i.e., adding vdW interactions and correcting self-interaction errors), it is not surprising

that different semi-local and hybrid functionals underbind bulk solids and yield increased

errors with increasing system size (nearest-neighbor distance, lattice constant, or nuclear

mass).

Performance of various density-functional approximations for cohesive properties of 64 bulk solids24

3.5. vdW interactions in bulk solids

As noted previously, one potential source of the size-related issues is the lack of a full

description of vdW interactions in the six functionals studied, particularly, the lack of

long-range vdW interactions, which form part of the correlation energy. The importance

of such interactions for bulk solids has become clearer in recent years. [82,96] In our own

previous study of six ionic and semiconductor solids, long-range vdW interactions were

included using C6 coefficients derived from accurate dielectric functions. The inclusion

of long-range vdW interactions on top of the PBE and HSE06 functionals lead to a

significant improvement for the cohesive properties of the six solids compared to the

results without vdW interactions, and as a result the characteristic underbinding of

PBE and HSE06 was largely remedied. [82]

Here we extend this study to 23 semiconductors, comprising all of the SC group

in the present study, apart from tin. The vdW interactions have been modelled using

the method proposed by Tkatchenko et al., [76] which accounts for both short-range

hybridization and long-range screening effects, seamlessly. As briefly discussed in

section 2.3, recent studies demonstrated that screening effects become important in

large molecules and materials. [72, 76, 77] Figure 9 shows the MAREs in the cohesive

properties (a0, E0, and B0) obtained for the 23 semiconductors using the six functionals

considered in the present study, alongside the results where three of the functionals are

augmented with long-range vdW interactions, specifically, PBE+vdW, M06-L+vdW,

and HSE06+vdW (corresponding data are shown in table SVIII). Employing PBE+vdW

leads to a consistent improvement in all three cohesive properties compared to PBE

alone, reducing deviations from experiment significantly, especially for the lattice

constants and bulk moduli. This is unsurprising, as the trends for PBE showed a size-

related dependence for the deviations from experiment, with PBE performing worse

for systems with heavier elements and, hence, larger lattice constants. As such larger

systems will have a larger contribution from vdW interactions, augmenting PBE with

a vdW term clearly and understandably leads to improvement.

Turning to HSE06, again, all three cohesive properties are in better agreement when

the functional is augmented with a vdW term. Overall, HSE06+vdW yields the most

accurate results among the DFT+vdW approaches employed, solving the underbinding

issue of HSE06, and in fact leads to slight overbinding, with overestimation of both

cohesive energies and bulk moduli. In contrast, augmenting M06-L with a vdW term

improves lattice constants and bulk moduli but worsens the MARE in the cohesive

energies, and as a result gives mixed performance. This likely stems from the fact that

the functional form of M06-L contains many empirical parameters that are determined

through fits to molecular data. This will partly capture some vdW interactions, but

effects and contributions outside or beyond the data set will not be captured, leading

to limited transferability. Similar to M06-L, the ability to capture some mid-range

vdW interactions of SCAN, which has been seen from the improved performance on

e.g., the S22 set [34] and the bulk solids in this work, makes it difficult to further

Performance of various density-functional approximations for cohesive properties of 64 bulk solids25

develop DFT+vdW methods. One of our co-authors [97] has recently illustrated this

particular issue of coupling vdW interactions with semi-local functionals, and they

pointed out the effective range (at which distance fluctuations are correlated) of SCAN

depends on system size. Capturing new or higher-level contributions will always be a

challenge for empirical functionals (MGGAs or GGAs). Developing new functionals and

augmenting existing ones with physically motivated contributions, such as long-range

vdW interactions, may often be easier starting from a non-empirical functional that is

not fitted to specific types of systems or interactions.

Figure 9. The mean absolute relative error (MARE, %) obtained within LDA,

PBEsol, PBE, PBE+vdW, M06-L, M06-L+vdW, SCAN, HSE06, and HSE06+vdW

compared to experimental data for the lattice constants a0, cohesive energies E0, and

bulk moduli B0, as an average over 23 semiconductor solids (including groups IVA,

IIIA-VA, and IIB-VIA).

4. Conclusions

In this work the cohesive properties of 64 solids have been studied using density-

functional approximations from rungs 1–4 of Jacob’s ladder (LDA, GGA, MGGA, and

hybrid functionals). As a precursor to comparing the calculated values to experiment,

the importance of zero-point vibrational contributions has been explored and found to

be significant for certain solids and properties, with the bulk moduli, in particular, have

a larger contribution from ZPE than lattice constants or cohesive energies.

For the cohesive properties, the present study broadly reproduces the well-known

trends of the LDA and PBE functionals. LDA delivers fairly good predictions on

the lattice constants and bulk moduli of covalently-bonded systems, however, the

Performance of various density-functional approximations for cohesive properties of 64 bulk solids26

cohesive energies are considerably overestimated with a MARE of ∼20%. PBE predicts

overall accurate cohesive energies for a diverse type of crystals and for metals and

transition-metal carbides and nitrides the improvement over other existing functionals

is pronounced. While PBE underbinds significantly, PBEsol and HSE06 both improve

on this, with PBEsol overbinding and HSE06 underbinding but to a lessor extent than

PBE. In comparison, the MGGA M06-L gives a better description than PBE for certain

semiconductors and ionic crystals, but yields poor prediction of bulk moduli, while the

SCAN functional is superior for the description of cohesion in non-metallic solids.

By comparing the DFT results to experimental studies and empirical observations,

trends in the relationships between pairs of cohesive properties have been explored

with all six functionals being able to broadly reproduced the experimental trends.

However, systematic differences are observed in the deviations of the DFT results from

the experimental data. As the experimental trends point to a clear relationship between

the lattice constant and both the bulk modulus and the cohesive energy, it would be

expected therefore, for deviations of the bulk moduli and the cohesive energies to be

inversely related to those of the lattice constants. The PBE functional reproduces this

behavior better than other functionals, suggesting that PBE has clear and systematic

reasons for its deviations from experiment.

Overall, none of the functionals tested here can be considered as a universal method

that is better than the others when applied to a broad range of solids. Considering the

trends in deviations for different classes of solids and different quantities (and between

different quantities) can be fruitful for developing new DFAs. It is noticeable that

deviations from experiment increase for a number of functionals with larger unit-cell

sizes (and hence heavier atoms). Undoubtedly, some of the deviation stems from the

lack of long-range vdW interactions in these functionals, which will be more significant

for heavier atoms. For 23 semiconductors, augmenting the PBE and HSE06 functionals

with a vdW correction leads to consistent improvements. However, augmenting the

empirical MGGA M06-L leads to improvements in lattice constants and bulk moduli,

but worsens cohesive energies. The current work reinforces the need to go beyond (semi-

)local approaches for obtaining accurate cohesive properties of bulk solids. It can also be

concluded that some of the deviation stems from the lack of long-range vdW interactions.

PBE represents a natural starting point to add such long-range vdW interactions, as its

deviations from experiment are systematic and more consistent than other functionals,

and also because of its computational efficiency.

Acknowledgements

A.T. acknowledges support from the European Research Council (ERC Consolidator

Grant BeStMo). G.X.Z. would like to acknowledge support from the National Natural

Science Foundation of China (Grant No. 21503057) and the Fundamental Research

Funds for the Central Universities (Grant No. HIT.NSRIF.2017032).

Performance of various density-functional approximations for cohesive properties of 64 bulk solids27

References

[1] Hohenberg P and Kohn W 1964 Phys. Rev. 136 B864

[2] Kohn W and Sham L J 1965 Phys. Rev. 140 A1133

[3] Perdew J P, Ruzsinszky A, Tao J, Staroverov V, Scuseria G and Csonka G 2005 J. Chem. Phys.

123 062201

[4] Cohen A J, Mori-Sanchez P and Yang W 2012 Chem. Phys. 112 289

[5] Burke K 2012 J. Chem. Phys. 136 150901

[6] Cohen A J, Mori-Sanchez P and Yang W 2008 Science 321 792

[7] Becke A D 2014 J. Chem. Phys. 140 18A301

[8] Staroverov V N, Scuseria G E, Tao J and Perdew J P 2004 Phys. Rev. B 69 075102

[9] Staroverov V N, Scuseria G E, Tao J and Perdew J P 2008 Phys. Rev. B 78 239907(E)

[10] Haas P, Tran F and Blaha P 2009 Phys. Rev. B 79 085104

[11] Haas P, Tran F and Blaha P 2009 Phys. Rev. B 79 209902(E)

[12] Csonka G I, Perdew J P, Ruzsinszky A, Philipsen P H T, Lebegue S, Paier J, Vydrov O A and

Angyan J G 2009 Phys. Rev. B 79 155107

[13] Sun J, Marsman M, Csonka G I, Ruzsinszky A, Hao P, Kim Y S, Kresse G and Perdew J P 2011

Phys. Rev. B 84 035117

[14] Schimka L, Harl J and Kresse G 2011 J. Chem. Phys. 134 024116

[15] Tran F, Laskowski R, Blaha P and Schwarz K 2007 Phys. Rev. B 75 115131

[16] Haas P, Tran F, Blaha P, Pedrora L S, Silva A J R, Odashima M M and Capelle K 2010 Phys.

Rev. B 81 125136

[17] Hao P, Fang Y, Sun J, Csonka G I, Philipsen P H T and Perdew J P 2012 Phys. Rev. B 85 014111

[18] Mattsson A E, Armiento R, Paier J, Kresse G, Wills J M and Mattsson T 2008 J. Chem. Phys

128 084714

[19] Tran F, Stelzl J and Blaha P 2016 J. Chem. Phys. 144 204120

[20] Lejaeghere K, Bihlmayer G, Bjrkman T, Blaha P, Blgel S, Blum V, Caliste D, Castelli I E, Clark

S J, Corso A D, Gironcoli S d, Deutsch T, Dewhurst J K, Marco I D, Draxl C, Duak M, Eriksson

O, Flores-Livas J A, Garrity K F, Genovese L, Giannozzi P, Giantomassi M, Goedecker S, Gonze

X, Grns O, Gross E K U, Gulans A, Gygi F, Hamann D R, Hasnip P J, Holzwarth N A W, Iuan

D, Jochym D B, Jollet F, Jones D, Kresse G, Koepernik K, Kkbenli E, Kvashnin Y O, Locht

I L M, Lubeck S, Marsman M, Marzari N, Nitzsche U, Nordstrm L, Ozaki T, Paulatto L, Pickard

C J, Poelmans W, Probert M I J, Refson K, Richter M, Rignanese G M, Saha S, Scheffler M,

Schlipf M, Schwarz K, Sharma S, Tavazza F, Thunstrm P, Tkatchenko A, Torrent M, Vanderbilt

D, Setten M J v, Speybroeck V V, Wills J M, Yates J R, Zhang G X and Cottenier S 2016

Science 351 aad3000

[21] Perdew J P and Schmidt K 2001 in Density Functional Theory and Its Application to Materials

(AIP, Melville, New York)

[22] Perdew J P, Burke K and Ernzerhof M 1996 Phys. Rev. Lett. 77 3865

[23] Zhang Y and Yang W 1998 Phys. Rev. Lett. 80 890

[24] Hammer B, Hansen L B and Nørskov J K 1999 Phys. Rev. B 59 7413

[25] Perdew J P, Ruzsinszky A, Csonka G I, Vydrov O A, Scuseria G E, Constantin L A, Zhou X and

Burke K 2008 Phys. Rev. Lett. 100 136406

[26] Ghosh S K and Parr R G 1986 Phys. Rev. A 34 785

[27] Becke A D and Roussel M E 1989 Phys. Rev. A 39 3761

[28] Tao J, Perdew J P, Staroverov V N and Scuseria G E 2003 Phys. Rev. Lett. 91 146401

[29] Wellendorff J, Lundgaard K T, Jacobsen K W and Bligaard T 2014 J. Chem. Phys 140 144107

[30] Xiao B, Sun J, Ruzsinszky A, Feng J, Haunschild R, Scuseria G E and Perdew J P 2013 Phys.

Rev. B 88 184103

[31] Staroverov V N, Scuseria G E, Tao J and Perdew J P 2003 J. Chem. Phys. 119 12129

[32] Perdew J P, Ruzsinszky A, Csonka G I, Constantin L A and Sun J 2009 Phys. Rev. Lett. 103

Performance of various density-functional approximations for cohesive properties of 64 bulk solids28

026403

[33] Perdew J P, Ruzsinszky A, Csonka G I, Constantin L A and Sun J 2011 Phys. Rev. Lett. 106

179902(E)

[34] Sun J, Ruzsinszky A and Perdew J P 2015 Phys. Rev. Lett. 115 036402

[35] Brandenburg J G, Bates J E, Sun J and Perdew J P 2016 Phys. Rev. B 94 115144

[36] Peng H, Yang Z H, Sun J and Perdew J P 2016 Phys. Rev. X 6 041005

[37] Perdew J P, Sun J, Ruzsinszky A, Mezei P D and Csonka G I 2016 Period. Polytech. Chem. Eng.

60 2

[38] Sun J, Remsing R C, Zhang Y, Sun Z, Ruzsinszky A, Peng H, Yang Z, Raul A, Waghmare U, Wu

X, Klein M L and Perdew J P 2016 Nat. Chem. 8 831

[39] Becke A D 1993 J. Chem. Phys. 98 1372

[40] Becke A D 1993 J. Chem. Phys. 98 5648

[41] Heyd J, Scuseria G E and Ernzerhof M 2003 J. Chem. Phys. 118 8207

[42] Heyd J, Scuseria G E and Ernzerhof M 2006 J. Chem. Phys. 124 219906(E)

[43] Heyd J and Scuseria G E 2004 J. Chem. Phys. 121 1187

[44] Heyd J, Peralta J E, Scuseria G E and Martin R L 2005 J. Chem. Phys. 123 174101

[45] Henderson T M, Paier J and Scuseria G E 2011 Phys. Status Solidi B 248 767

[46] Vydrov O A and Scuseria G E 2006 J. Chem. Phys. 125 234109

[47] Krukau A V, Vydrov O A, Izmaylov A F and Scuseria G E 2006 J. Chem. Phys. 125 224106

[48] Paier J, Marsman M, Hummer K, Kresse G, Gerber I C and Angyan J G 2006 J. Chem. Phys.

124 154709

[49] Paier J, Marsman M and Kresse G 2007 J. Chem. Phys. 127 024103

[50] Marsman M, Paier J, Stroppa A and Kresse G 2008 J. Phys.: Condens. Matter 20 064201

[51] Verma P and Truhlar D G 2017 J. Phys. Chem. Lett. 8 380

[52] Furche F and Perdew J P 2006 J. Chem. Phys 124 044103

[53] Harl J, Schimka L and Kresse G 2010 Phys. Rev. B 81 115126

[54] Ren X, Rinke P, Joas C and Scheffler M 2012 J. Mater. Sci. 47 7447

[55] Eshuis H, Bates J E and Furche F 2012 Theor. Chem. Acc. 131 1084

[56] Ren X, Tkatchenko A, Rinke P and Scheffler M 2011 Phys. Rev. Lett. 106 153003

[57] Grabowski B, Hickel T and Neugebauer J 2007 Phys. Rev. B 76 024309

[58] Yin M T and Cohen M L 1981 Phys. Rev. B 24 6121

[59] Yin M T and Cohen M L 1982 Phys. Rev. B 26 5668

[60] Zhao Y and Truhlar D G 2006 J. Chem. Phys. 125 194101

[61] Zhao Y and Truhlar D G 2008 J. Chem. Phys. 128 184109

[62] Peverati R and Truhlar D G 2012 J. Chem. Phys. 136 134704

[63] See supplementary material

[64] Blum V, Gehrke R, Hanke F, Havu P, Havu V, Ren X, Reuter K and Scheffler M 2009 Comput.

Phys. Commun. 180 2175

[65] Birch F 1947 Phys. Rev. 71 809

[66] Monkhorst H J and Pack J D 1976 Phys. Rev. B 13 5188

[67] van Lenthe E, Baerends E J and Snijders J G 1994 J. Chem. Phys. 101 9783

[68] Philipsen P H T and Baerends E J 2000 Phys. Rev. B 61 1773

[69] Grimme S 2011 WIREs Rev. Comput. Mol. Sci. 1 211

[70] Johnson E R, Mackie I D and DiLabio G A 2009 J. Phys. Org. Chem. 22 1127

[71] Klimes J and Michaelides A 2012 J. Chem. Phys. 137 120901

[72] Hermann J, DiStasio Jr R A and Tkatchenko A 2017 Chem. Rev. 117 4714

[73] Tkatchenko A and Scheffler M 2009 Phys. Rev. Lett. 102 073005

[74] Hirshfeld F L 1977 Theor. Chim. Acta. 44 129

[75] Chu X and Dalgarno A 2004 J. Chem. Phys. 121 4083

[76] Tkatchenko A, DiStasio Jr R A, Car R and Scheffler M 2012 Phys. Rev. Lett. 108 236402

[77] Reilly A M and Tkatchenko A 2015 Chem. Sci. 6 3289

Performance of various density-functional approximations for cohesive properties of 64 bulk solids29

[78] Togo A, Oba F and Tanaka I 2008 Phys. Rev. B 78 134106

[79] https://atztogo.github.io/phonopy/fhi-aims.html.

[80] Kern G, Kresse G and Hafner J 1999 Phys. Rev. B 59 8551

[81] Alchagirov A B, Perdew J P, Boettger J C, Albers R C and Fiolhais C 2001 Phys. Rev. B 63

224115

[82] Zhang G X, Tkatchenko A, Paier J, Appel H and Scheffler M 2011 Phys. Rev. Lett. 107 245501

[83] Kresse G and Furthmuller J 1996 Comput. Mater. Sci. 6 15

[84] Kresse G and Furthmuller J 1996 Phys. Rev. B 54 11169

[85] Janthon P, M K S, Vines F, Limtrakul J and Illas F 2013 J. Chem. Theory Comput. 9 1631

[86] Anderson O L and Nafe J E 1965 J. Geophys. Res. 70 3950

[87] Cohen M L 1985 Phys. Rev. B 32 7988

[88] Lam P K and Cohen M L 1987 Phys. Rev. B 35 9190

[89] Schlosser H 1992 J. Phys. Chem. Solids 53 855

[90] Schlosser H 1993 Phys. Status Solidi B 179 K1

[91] Aresti A, Garbato L and Rucci A 1984 J. Phys. Chem. Solids 45 361

[92] Dzivenko D, Zerr A, Guignot N, Mezouar M and Riedel R 2010 Euro. Phys. Lett. 92 66001

[93] Korir K K, Amolo G O, Makau N W and Joubert D P 2011 Diam. Relat. Mater. 20 157

[94] Schimka L, Klimes J, Marsman M and Kresse G 2013 Phys. Rev. B 87 214102

[95] Hui K and Chai J 2016 J. Chem. Phys. 144 044114

[96] Klimes J, Bowler D R and Michaelides A 2011 Phys. Rev. B 83 195131

[97] Hermann J and Tkatchenko A 2018 J. Chem. Theory Comput. 14 1361